We need your consent to use the individual data so that you can see information about your interests, among other things. Click "OK" to give your consent.
Standard Test Method for Facesheet Properties of Sandwich Constructions by Long Beam FlexureTranslate name
STANDARD published on 1.2.2020
Designation standards: ASTM D7249/D7249M-20
Publication date standards: 1.2.2020
The number of pages: 10
Approximate weight : 30 g (0.07 lbs)
Country: American technical standard
Category: Technical standards ASTM
bending stress, facesheet modulus, facesheet strength, facesheet stress, flexural stiffness, sandwich construction, sandwich deflection,, ICS Number Code 79.060.01 (Wood-based panels in general)
|Significance and Use|
5.1 Flexure tests on flat sandwich construction may be conducted to determine the sandwich flexural stiffness, the core shear strength, and shear modulus, or the facesheets’ compressive and tensile strengths. Tests to evaluate core shear strength may also be used to evaluate core-to-facesheet bonds.
5.2 This test method is limited to obtaining the strength and stiffness of the sandwich panel facesheets, and to obtaining load-deflection data for use in calculating sandwich beam flexural and shear stiffness using Practice . Due to the curvature of the flexural test specimen when loaded, facesheet compression strength from this test may not be equivalent to the facesheet compression strength of sandwich structures subjected to pure edgewise (in-plane) compression.
5.3 Core shear strength and shear modulus are best determined in accordance with Test Method provided bare core material is available. Test Method may also be used to determine core shear strength. Practice may be used to calculate the flexural and shear stiffness of sandwich beams.
5.4 This test method can be used to produce facesheet strength data for structural design allowables, material specifications, and research and development applications; it may also be used as a quality control test for bonded sandwich panels.
5.5 Factors that influence the facesheet strength and shall therefore be reported include the following: facesheet material, core material, adhesive material, methods of material fabrication, facesheet stacking sequence and overall thickness, core geometry (cell size), core density, adhesive thickness, specimen geometry, specimen preparation, specimen conditioning, environment of testing, specimen alignment, loading procedure, speed of testing, facesheet void content, adhesive void content, and facesheet volume percent reinforcement. Further, facesheet strength may be different between precured/bonded and co-cured facesheets of the same material.
Note 2: Concentrated forces on beams with thin facesheets and low density cores can produce results that are difficult to interpret, especially close to the failure point. Wider loading blocks and rubber pressure pads may assist in distributing the forces.
Note 3: To ensure that simple sandwich beam theory is valid, a good rule of thumb for the four-point bending test is the support span length divided by the sandwich thickness should be greater than 20 (1.1 This test method covers determination of facesheet properties of flat sandwich constructions subjected to flexure in such a manner that the applied moments produce curvature of the sandwich facesheet planes and result in compressive and tensile forces in the facesheets. Permissible core material forms include those with continuous bonding surfaces (such as balsa wood and foams) as well as those with discontinuous bonding surfaces (such as honeycomb).
1.2 Units—The values stated in either SI units or inch-pound units are to be regarded separately as standard. The values stated in each system are not necessarily exact equivalents; therefore, to ensure conformance with the standard, each system shall be used independently of the other, and values from the two systems shall not be combined.
1.2.1 Within the text, the inch-pound units are shown in brackets.
1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
Note 1: Alternate procedures for determining the compressive strength of unidirectional polymer matrix composites materials in a sandwich beam configuration may be found in Test Method .
1.4 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
|2. Referenced Documents|
Do you want to make sure you use only the valid technical standards?
We can offer you a solution which will provide you a monthly overview concerning the updating of standards which you use.
Would you like to know more? Look at this page.
Latest update: 2022-11-27 (Number of items: 2 642 910)
© Copyright 2022 NORMSERVIS s.r.o.